Generalized far-infrared magneto-optic ellipsometry for semiconductor layer structures: determination of free-carrier effective-mass, mobility, and concentration parameters in n-type GaAs
JOSA A, Vol. 20, Issue 2, pp. 347-356 (2003)
http://dx.doi.org/10.1364/JOSAA.20.000347
Acrobat PDF (252 KB)
Abstract
We report for the first time on the application of generalized ellipsometry at far-infrared wavelengths (wave numbers from 150 cm^{−1} to 600 cm^{−1}) for measurement of the anisotropic dielectric response of doped polar semiconductors in layered structures within an external magnetic field. Upon determination of normalized Mueller matrix elements and subsequent derivation of the normalized complex Jones reflection matrix r of an n-type doped GaAs substrate covered by a highly resistive GaAs layer, the spectral dependence of the room-temperature magneto-optic dielectric function tensor of n-type GaAs with free-electron concentration of 1.6× 10^{18} cm^{−3} at the magnetic field strength of 2.3 T is obtained on a wavelength-by-wavelength basis. These data are in excellent agreement with values predicted by the Drude model. From the magneto-optic generalized ellipsometry measurements of the layered structure, the free-carrier concentration, their optical mobility, the effective-mass parameters, and the sign of the charge carriers can be determined independently, which will be demonstrated. We propose magneto-optic generalized ellipsometry as a novel approach for exploration of free-carrier parameters in complex organic or inorganic semiconducting material heterostructures, regardless of the anisotropic properties of the individual constituents.
© 2003 Optical Society of America
OCIS Codes
(260.1180) Physical optics : Crystal optics
(260.2130) Physical optics : Ellipsometry and polarimetry
(260.3090) Physical optics : Infrared, far
Citation
Mathias Schubert, Tino Hofmann, and Craig M. Herzinger, "Generalized far-infrared magneto-optic ellipsometry for semiconductor layer structures: determination of free-carrier effective-mass, mobility, and concentration parameters in n-type GaAs," J. Opt. Soc. Am. A 20, 347-356 (2003)
http://www.opticsinfobase.org/josaa/abstract.cfm?URI=josaa-20-2-347
Sort: Year | Journal | Reset
References
- The effective-mass concept addressed here descends from the similarity with the Newton force equation (acceleration of a body with mass m) and the acceleration experienced by a Bloch electron due to an external force. The inverse tensor obtained thereby depends on the curvature of the plots of electron energetic states versus electron momentum, which is diagonal by a suitable choice of axes. Different experiments require different concepts, resulting in definition of the effective conductivity mass, the density-of-states effective mass, the Hall effective mass, or the cyclotron effective mass, all of which are not discussed here. For the material investigated here (GaAs), the response of the zinc-blended, Γ-point conduction band (single-species, i.e., single-valley) Bloch electrons studied at infrared wavelengths is on a time scale much smaller than the average time between scattering events of the free electrons. One may also refer to the effective mass here as an (infrared) optical effective mass. See also Refs. 2 and 3.
- C. M. Wolfe, N. Holonyak, Jr., and G. E. Stillmann, Physical Properties of Semiconductors (Prentice-Hall, Englewood Cliffs, N.J., 1989).
- C. R. Pidgeon, “Free carrier optical properties of semiconductors,” in Handbook of Semiconductors, M. Balkanski, ed. (North-Holland, Amsterdam, 1980), Vol. 2, pp. 223–228.
- P. Drude, The Theory of Optics, translated from German by C. R. Mann and R. A. Millikan (Longmans, Green, New York, 1902).
- H. Raether, Surface Polaritons (Springer, Berlin, 1988).
- A. Röseler, Infrared Spectroscopic Ellipsometry (Akademie, Berlin, 1992).
- J. J. Brion, R. F. Wallis, A. Hartstein, and E. Burstein, “Theory of magnetoplasmons in semiconductors,” Phys. Rev. Lett. 28, 1455–1458 (1972).
- J. J. Brion, R. F. Wallis, A. Hartstein, and E. Burstein, “Interaction of surface magnetoplasmons and surface optical phonons in polar semiconductors,” Surf. Sci. 34, 73–80 (1973).
- A. Hartstein, E. Burstein, J. J. Brion, and R. F. Wallis, “Surface polaritons on semi-infinite anisotropic media,” Surf. Sci. 34, 81–89 (1973).
- R. F. Wallis, J. J. Brion, E. Burstein, and A. Hartstein, “Theory of surface polaritons in anisotropic dielectric media with application to surface magnetoplasmons in semiconductors,” Phys. Rev. B 9, 3424–3437 (1974).
- M. Schubert, “Infrared ellipsometry on III-V semiconductor layer structures,” Habilitationsschrift (Universität Leipzig, Leipzig, Germany), available at http://www.uni-leipzig.de/~hlp/ellipsometrie.
- G. B. Wright and B. Lax, “Magnetoreflection experiments in intermetallics,” J. Appl. Phys. 32, 2113–2117 (1961).
- M. Cardona, “Electron effective masses of InAs and GaAs as a function of temperature and doping,” Phys. Rev. 121, 752–758 (1961).
- Restrictions apply to highly conductive layers that are optically thick, such as highly doped semiconductor substrates, or metal films several hundreds of nanometers thick. As long as the layer with high free-carrier concentration is passing electromagnetic radiation on to the next constituent, the ellipsometric parameters will contain information about the buried layers.
- R. M. A. Azzam and N. M. Bashara, Ellipsometry and Polarized Light (North-Holland, Amsterdam, 1984).
- D. E. Aspnes, “The accurate determination of optical properties by ellipsometry,” in Handbook of Optical Constants of Solids, E. D. Palik, ed. (Academic, New York, 1998), Vol. I, pp. 89–112.
- R. M. A. Azzam and N. M. Bashara, “Generalized ellipsometry for surfaces with directional preference: application to diffraction gratings,” J. Opt. Soc. Am. 62, 1521–1523 (1972).
- M. Schubert, B. Rheinländer, B. Johs, C. M. Herzinger, and J. A. Woollam, “Extension of rotating analyzer ellipsometry to generalized ellipsometry: determination of the dielectric function tensor from uniaxial TiO_{2},” J. Opt. Soc. Am. A 13, 875–883 (1996).
- G. E. Jellison, Jr. and L. A. Boatner, “Optical functions of uniaxial ZnO determined by generalized ellipsometry,” Phys. Rev. B 58, 3586–3589 (1998).
- D. W. Thompson, M. J. De Vries, T. E. Tiwald, and J. A. Woollam, “Determination of optical anisotropy in calcite from ultraviolet to mid-infrared by generalized ellipsometry,” Thin Solid Films 313–314, 341–346 (1998).
- M. Schubert, T. E. Tiwald, and J. A. Woollam, “Explicit solutions for the optical properties of arbitrary magneto-optic materials in generalized ellipsometry,” Appl. Opt. 38, 177–187 (1999).
- M. Schubert and C. M. Herzinger, “Ellipsometry on anisotropic materials: Bragg conditions and phonons in dielectric helical thin films,” Phys. Status Solidi A 188, 1563–1575 (2001).
- M. Schubert and W. Dollase, “Generalized ellipsometry for biaxial absorbing minerals: determination of crystal orientation and optical constants from Sb_{2}S_{3},” Opt. Lett. 27, 2073–2075 (2002).
- M. Schubert, “Theory and application of generalized ellipsometry,” in Handbook of Ellipsometry, G. E. Irene and H. W. Tompkins, eds. (to be published).
- M. Schubert, B. Rheinländer, B. Johs, and J. A. Woollam, “Application of generalized ellipsometry to complex optical systems,” in Polarimetry and Ellipsometry, M. Pluta and T. R. Wolinsky, eds., Proc. SPIE 3094, 255–265 (1997).
- M. Schubert, “Generalized ellipsometry and complex optical systems,” Thin Solid Films 313–314, 323–332 (1998).
- M. Schubert, A. Kasic, T. Hofmann, V. Gottschalch, J. Off, F. Scholz, E. Schubert, H. Neumann, I. J. Hodgkinson, M. D. Arnold, W. A. Dollase, and C. M. Herzinger, “Generalized ellipsometry of complex mediums in layered systems,” in Complex Mediums III: Beyond Linear Isotropic Dielectrics, A. Lakhtakia, G. Dewar, and M. W. McCall, eds., Proc. SPIE 4806, 264–276 (2002).
- This set comprises six real-valued quantities out of the eight possible values contained within the Jones matrix—lacking the light beam’s absolute intensity and absolute phase information. For a definition of the Jones matrix elements, see Refs. 15, 17, 18, 24 25 26 27, and references therein.
- G. E. Jellison, Jr., “Spectroscopic ellipsometry data analysis: measured versus calculated quantities,” Thin Solid Films 313–314, 33–39 (1998).
- C. M. Herzinger, P. G. Snyder, B. Johs, and J. A. Woollam, “InP optical constants between 0.75 and 5.0 eV determined by variable-angle spectroscopic ellipsometry,” J. Appl. Phys. 77, 1715–1724 (1995).
- M. Schubert, “Polarization-dependent optical parameters of arbitrarily anisotropic homogeneous layered systems,” Phys. Rev. B 53, 4265–4274 (1996).
- T. E. Tiwald and M. Schubert, “Measurement of rutile TiO_{2} from 0.148 to 33 μm using generalized ellipsometry,” in Optical Diagnostic Methods For Inorganic Materials II, L. M. Hanssen, ed., Proc. SPIE 4103, 19–29 (2000).
- R. Henn, C. Bernhard, A. Wittlin, M. Cardona, and S. Uchida, “Far infrared ellipsometry using synchrotron radiation: the out-of-plane response of La_{2−x}Sr_{x}CuO_{4},” Thin Solid Films 313–314, 643–648 (1998).
- J. Kircher, R. Henn, M. Cardona, P. L. Richards, and G. P. Williams, “Far-infrared ellipsometry using synchrotron radiation,” J. Opt. Soc. Am. B 14, 705–712 (1997).
- J. Humlíček, R. Henn, and M. Cardona, “Infrared vibrations in LaSrGaO_{4} and LaSrAlO_{4},” Phys. Rev. B 61, 14554–14563 (2000).
- T. E. Tiwald, J. A. Woollam, St. Zollner, J. Christiansen, R. B. Gregory, T. Wetteroth, and S. R. Wilson, “Carrier concentration and lattice absorption in bulk and epitaxial silicon carbide determined using infrared ellipsometry,” Phys. Rev. B 60, 11464–11474 (1999).
- M. Schubert, T. E. Tiwald, and C. M. Herzinger, “Infrared dielectric anisotropy and phonon modes of sapphire,” Phys. Rev. B 61, 8187–8201 (2000).
- A. Kasic, M. Schubert, S. Einfeldt, D. Hommel, and T. E. Tiwald, “Free-carrier and phonon properties of n- and p-type hexagonal GaN films measured by infrared ellipsometry,” Phys. Rev. B 62, 7365–7377 (2000).
- C. Kittel, Introduction to Solid State Physics (Wiley, New York, 1985).
- In view of the generalized ellipsometry applications at oblique incidence, MO setups will be addressed as follows: the polar MO (PMO) setup with B parallel to the sample normal, the longitudinal MO (LMO) setup with B parallel to the sample surface and parallel to the plane of incidence, and the transverse MO (TMO) setup with B perpendicular to the sample normal and perpendicular to the plane of incidence. In the MO literature, different terms are in use: Near-normal-incidence reflection-type Kerr-effect measurements are referred to as transverse, longitudinal, and polar configurations, in conceptual agreement with the above notation. Faraday- and Voigt-effect measurements address transmission-type linear polarization rotation measurements in the above PMO and mixed LMO–TMO configurations, respectively. See Ref. 3 or Ref. 41. These configurations mostly result from the simplicity of the corresponding equations, which describe the polarized light reflection and transmission situations for the anisotropic materials. These requirements are now dispensed with because of the availability of explicit solutions for light propagation in arbitrarily nonsymmetric (MO) dielectric materials.21
- M. Mansuripur, The Physical Principles of Magneto-Optical Recording (Cambridge U. Press, Cambridge, UK, 1995).
- E. D. Palik, “Gallium arsenide (GaAs),” in Handbook of Optical Constants of Solids, E. D. Palik, ed. (Academic, New York, 1998), Vol. I; pp. 429–444.
- E. Burstein and F. De Martini, eds., Polaritons (Pergamon, New York, 1974).
- D. W. Berreman, “Infrared absorption at longitudinal optic frequency in cubic crystal films,” Phys. Rev. 130, 2193–2198 (1963).
- St. Zollner, J. P. Carrejo, T. E. Tiwald, and J. A. Woollam, “The origin of the Berreman effect in SiC homostructures,” Phys. Status Solidi B 208, R3–R4 (1998).
- J. Humlíček, “Infrared spectroscopy of LiF on Ag and Si,” Phys. Status Solidi B 215, 155–159 (1999).
- M. Schubert, B. Rheinländer, C. Cramer, H. Schmiedel, J. A. Woollam, B. Johs, and C. M. Herzinger, “Generalized transmission ellipsometry for twisted biaxial dielectric media: application to chiral liquid crystals,” J. Opt. Soc. Am. A 13, 1930–1940 (1996).
- A. Raymond, J. L. Robert, and C. Bernard, “The electron effective mass in heavily doped GaAs,” J. Phys. C 12, 2289–2293 (1979).
Cited By |
Alert me when this paper is cited |
OSA is able to provide readers links to articles that cite this paper by participating in CrossRef's Cited-By Linking service. CrossRef includes content from more than 3000 publishers and societies. In addition to listing OSA journal articles that cite this paper, citing articles from other participating publishers will also be listed.
« Previous Article | Next Article »
OSA is a member of CrossRef.